Version 1.0 2010.11.02 1 of 16
Course: Quality Assurance Module 6
Version 1.0 2010.11.02 2 of 16
Table of ContentsMODULE 6................................................................................................................................................3
Preheating, interpass and post heating to prevent hydrogen cracking ...........................................16 Preheat .................................................................................................................................. 16 Interpass and post heating..................................................................................................... 16
Version 1.0 2010.11.02 3 of 16
MODULE 6 Objective: Know the effect of welding in terms of shrinkage, residual stresses and distortion. And know how to minimise distortion before, during and after welding. Scope: The thermal cycle in welding Development of residual stresses due to solidification, cooling and shrinkage Effects of restraint on residual stress Significance of residual stress Preheating, postheating Relationship between heat input and shrinkage, residual stress and distortion. Development of distortion; effect of heat input, weld size, penetration, and number of runs single- and
double-sided fillet welded joints and in butt welds. Corrective measures, procedure, welding technique, sequence, joint preparation, pre-setting Correction of distortion after welding Expected results: Describe the thermal cycle during welding. Describe distortion resulting form shrinkage. Describe residual stresses. Name measures to minimise distortion. Describe the main causes for weld shrinkage. Outline the main effects on a weld due to residual stresses. Control over the weld distortion Beginning welders and even those that are more experienced commonly struggle with the problem of weld distortion, (warping of the base plate caused by heat from the welding arc). Distortion is troublesome for a number of reasons, but one of the most critical is the potential creation of a weld that is not structurally sound. This paper will help to define what weld distortion is and then provide a practical understanding of the causes of distortion, effects of shrinkage in various types of welded assemblies and how to control it, and finally look at methods for distortion control.
Distortion in a weld results from the expansion and contraction of the weld metal and adjacent base metal during the heating and cooling cycle of the welding process. Doing all welding on one side of a part will cause much more distortion than if the welds are alternated from one side to the other. During this heating and cooling cycle, many factors affect shrinkage of the metal and lead to distortion, such as physical and mechanical properties that change as heat is applied.
Version 1.0 2010.11.02 4 of 16
If we cut through a welded connection and investigate the material, we can, when simplifying, say that the connection contains three zones: A. The parent metal which is not influenced by the welding, here shown in brown colour. B. The heat affected zone, here shown in light blue colour C. The weld metal, here shown in blue colour. Zone B and C are of course not so clearly defined in reality because the mixing of molten material takes place and the structural transfer is a gradual change of structure, but for the understanding of the heat distortion itself this does not play a major role. When a metallic material is heated it will expand in all directions. We can illustrate this as shown in figure 1. The material elements can be visualized as a cube. Before the heating the cube will have a dimension/size as shown in blue. After heating the dimension /size will expand to the yellow boundaries.
Fig 1. A material with a given dimension/size is heated and it will expand in all directions. If a steel bar is uniformly heated while unrestrained, it will expand in all directions and return to its original dimensions on cooling. However, in welding the heating will be locally causing the surrounding cold material to limit the free thermal expansion. In figure 2 this is illustrated by showing blue arrows, or forces , that will limit the free movement of the material.
Version 1.0 2010.11.02 5 of 16
Fig 2. The material will try to expand in all direction during heating. However the cold surrounding material will try to limit the expansion. It is restrained, during heating, and will have a limited expansion. On cooling, the deformed bar contracts uniformly, and is permanently deformed. The forces of the surrounding material will cause the internal material structure to be pressed together during the heating process. Or we may say that the distance between the smallest structural material elements will be reduced. When the material then cool down, the distance between the smallest structural elements will be kept, causing the cube to be shortened as shown in the white cube in figure 3.
Fig 3. When cooling down the original material will be shortend of the external forces from the cold material which press the expanded material together. The resulting cold dimension/size is here shown in white. However, during the cooling process, the hot material will will shrink and try to drag the surrounding cold material in the direction it shrinks. The surrounding material must then follow , unless it cracks, causing deformations to appear. In a welded joint, these same expansion and contraction forces act on the weld metal and on the base metal. As the weld metal solidifies and fuses with the base metal, it is in its maximum expanded from. On cooling, it attempts to contract to the volume it would normally occupy at the lower temperature, but it is restrained from doing so by the adjacent base metal. Because of this, stresses develop within the weld and the adjacent base metal. At this point, the weld stretches (or yields) and thins out, thus adjusting to the volume requirements of the
Version 1.0 2010.11.02 6 of 16
lower temperature. But only those stresses that exceed the yield strength of the weld metal are relieved by this straining. By the time the weld reaches room temperature - assuming complete restraint of the base metal so that it cannot move - the weld will contain locked-in tensile stresses approximately equal to the yield strength of the metal. If the restraints (clamps that hold the workpiece, or an opposing shrinkage force) are removed, the residual stresses are partially relieved as they cause the base metal to move, thus distorting the weldment.
The result will be that very strong forces appears and drag the cold material in the direction of the heated zone and we will consequently get a heat deformation.
Fig 4. The figure shows how much steel will expand when it is heated from 0 degree to 600 degrees.
Version 1.0 2010.11.02 7 of 16
Fig 5. Fillet weld. During heating the forces will go in the direction of the yellow arrows. However the reaction forces from the cold material will cause the molten structure to shrink. The cold material gives reaction forces as shown with the blue arrows. Cooling down causes the material to bend as shown in figure 6. V
Fig 6. The geometrical form of the fillet weld after cooling down. A butt weld gives the same problem as we had in a fillet weld. When heating the molten material will try to expand in the direction of the yellow arrows. Due to the reaction forces from the cold material the size of the molten material will shrink during the cooling process. The final result when the material cools down is that the surrounding cold material will be bent in the direction of the blue arrows.
Version 1.0 2010.11.02 8 of 16
Fig 7. A butt weld. During the cooling process the material will bend in the direction of the blue arrows. The design of the bevel causes more molten metal in the top of the bevel than in the bottom of the bevel, resulting in stronger contracting forces at the top. If we draw this in another perspective, the plate will look like this.
Fig 8. We see a straight surface, indicated by the dotted line. We also clearly see how the edges of the plate have been moved upwards caused by the forces earlier described.. In more complex designs and structures, you have to evaluate the heat distortion of each element and see how these elements fits together.
Version 1.0 2010.11.02 9 of 16
Fig 9. In this T-joint we see that the flange is bent as shown in the previous figures. In addition the leg will get a separate heat distortion and bed as shown. The resulting forces will create a structure as shown here in this drawing.
Fig 10. The figure shows the results of the heating of the material just at the end of the welding process. We see that the root opening has increased dramatically due to the heat influence.
Version 1.0 2010.11.02 10 of 16
Fig 11. This photo is the same as fig 10, but show the joint connection after the cooling. We see that the bevel opening has been completely closed. This is due to the contracting forces during the cooling process. For buttering and cladding the forces will be the same as for a standard butt weld. After welding with heat input followed by the cooling process, the material will be bent in the direction of the blue arrow.
Fig 12. A cold weld where we see that the heat from the welding process goes in the direction of the white arrow. The consequtive cooling process causes the material to bend in the direction of the blue arrows.
Version 1.0 2010.11.02 11 of 16
Fig 13. A photo of a clad weld as